#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/76/7027688.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_7027688
loop_
_publ_author_name
'Goodgame, David M. L.'
'Hussain, Izhar'
'White, Andrew J. P.'
'Williams, David J.'
_publ_section_title
;
 Synthesis and structure of a copper(II) melamine complex,
 [Cu(C3H6N6)(μ-OCH3)(ONO2)(HOCH3)]2, with direct Cu--melamine
 coordination
;
_journal_issue                   17
_journal_name_full
'Journal of the Chemical Society, Dalton Transactions'
_journal_page_first              2899
_journal_paper_doi               10.1039/a905576b
_journal_year                    1999
_chemical_formula_sum            'C10 H26 Cu2 N14 O10'
_chemical_formula_weight         629.53
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                89.938(3)
_cell_angle_beta                 81.778(5)
_cell_angle_gamma                70.111(5)
_cell_formula_units_Z            1
_cell_length_a                   7.8614(7)
_cell_length_b                   7.9384(5)
_cell_length_c                   10.4874(6)
_cell_measurement_reflns_used    41
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.85
_cell_measurement_theta_min      9.71
_cell_volume                     608.33(8)
_computing_cell_refinement       'Siemens XSCANS'
_computing_data_collection       'Siemens XSCANS'
_computing_data_reduction        'Siemens SHELXTL'
_computing_molecular_graphics    'Siemens SHELXTL'
_computing_publication_material  'Siemens SHELXTL'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       'Siemens P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0231
_diffrn_reflns_av_sigmaI/netI    0.0211
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2119
_diffrn_reflns_theta_max         62.99
_diffrn_reflns_theta_min         4.26
_diffrn_standards_interval_count 97
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    2.847
_exptl_absorpt_correction_T_max  0.5512
_exptl_absorpt_correction_T_min  0.3082
_exptl_absorpt_correction_type   Ellipsoidal
_exptl_crystal_colour            Blue
_exptl_crystal_density_diffrn    1.718
_exptl_crystal_description       rhombs
_exptl_crystal_F_000             322
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.37
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.250
_refine_diff_density_min         -0.580
_refine_diff_density_rms         0.065
_refine_ls_extinction_coef       0.0123(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   1.120
_refine_ls_goodness_of_fit_obs   1.133
_refine_ls_matrix_type           full
_refine_ls_number_parameters     192
_refine_ls_number_reflns         1940
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.443
_refine_ls_restrained_S_obs      1.130
_refine_ls_R_factor_all          0.0446
_refine_ls_R_factor_obs          0.0357
_refine_ls_shift/esd_max         0.005
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0411P)²+0.8361P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1194
_refine_ls_wR_factor_obs         0.0918
_reflns_number_observed          1859
_reflns_number_total             1957
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            905576bsup1.cif
_cod_data_source_block           DMLG9803
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0411P)^2^+0.8361P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0411P)^2^+0.8361P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        608.33(7)
_cod_original_sg_symbol_H-M      P-1
_cod_original_formula_sum        'C10 H26 N14 O10 Cu2'
_cod_database_code               7027688
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
Cu Cu 0.04806(6) -0.00565(5) 0.13377(4) 0.0266(2) Uani 1 d .
N1 N 0.2471(3) -0.1827(3) 0.2153(2) 0.0275(5) Uani 1 d .
C2 C 0.4234(4) -0.2199(4) 0.1569(3) 0.0297(7) Uani 1 d .
N2 N 0.4497(4) -0.1841(4) 0.0329(3) 0.0429(7) Uani 1 d D
H2A H 0.5680(16) -0.2200(52) -0.0033(36) 0.054(12) Uiso 1 d D
H2B H 0.3570(35) -0.1584(52) -0.0135(32) 0.049(11) Uiso 1 d D
N3 N 0.5700(3) -0.2867(4) 0.2159(3) 0.0337(6) Uani 1 d .
C4 C 0.5360(4) -0.3416(4) 0.3350(3) 0.0327(7) Uani 1 d .
N4 N 0.6778(4) -0.4117(5) 0.3982(3) 0.0504(8) Uani 1 d D
H4A H 0.6529(62) -0.4724(55) 0.4667(28) 0.071(14) Uiso 1 d D
H4B H 0.7928(23) -0.4378(63) 0.3568(39) 0.072(15) Uiso 1 d D
N5 N 0.3703(4) -0.3293(4) 0.3971(2) 0.0341(6) Uani 1 d .
C6 C 0.2299(4) -0.2430(4) 0.3362(3) 0.0287(7) Uani 1 d .
N6 N 0.0619(4) -0.2128(4) 0.3982(3) 0.0412(7) Uani 1 d D
H6A H -0.0323(33) -0.1637(47) 0.3546(32) 0.046(11) Uiso 1 d D
H6B H 0.0457(56) -0.2419(54) 0.4809(12) 0.056(12) Uiso 1 d D
O7 O -0.2260(3) -0.0534(3) 0.2393(2) 0.0442(6) Uani 1 d D
H7 H -0.2672(51) -0.1391(37) 0.2145(38) 0.052(12) Uiso 1 d D
C7 C -0.3694(6) 0.0872(7) 0.3139(5) 0.0623(12) Uani 1 d .
H7A H -0.4182(6) 0.0395(7) 0.3890(5) 0.093 Uiso 1 d R
H7B H -0.4645(6) 0.1405(7) 0.2630(5) 0.093 Uiso 1 d R
H7C H -0.3225(6) 0.1766(7) 0.3401(5) 0.093 Uiso 1 d R
O8 O 0.0915(3) -0.1583(3) -0.0196(2) 0.0322(5) Uani 1 d .
C8 C 0.1168(7) -0.3425(5) -0.0145(4) 0.0589(12) Uani 1 d .
H8A H 0.1900(7) -0.3933(5) 0.0511(4) 0.088 Uiso 1 d R
H8B H 0.1777(7) -0.4022(5) -0.0965(4) 0.088 Uiso 1 d R
H8C H -0.0001(7) -0.3575(5) 0.0054(4) 0.088 Uiso 1 d R
N9 N 0.1171(4) 0.2562(4) 0.2616(3) 0.0377(7) Uani 1 d .
O10 O -0.0019(3) 0.1780(3) 0.2771(2) 0.0330(5) Uani 1 d .
O11 O 0.2353(4) 0.2131(4) 0.1654(3) 0.0558(7) Uani 1 d .
O12 O 0.1056(5) 0.3719(5) 0.3436(3) 0.0772(10) Uani 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu -1.9646 0.5888 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O8 Cu O8 78.10(9) 2 .
O8 Cu O10 95.32(9) 2 .
O8 Cu O10 172.67(9) . .
O8 Cu N1 165.09(10) 2 .
O8 Cu N1 93.88(9) . .
O10 Cu N1 91.81(10) . .
O8 Cu O7 90.86(9) 2 .
O8 Cu O7 98.15(9) . .
O10 Cu O7 85.07(9) . .
N1 Cu O7 102.81(9) . .
O8 Cu Cu 39.07(6) 2 2
O8 Cu Cu 39.03(6) . 2
O10 Cu Cu 134.31(7) . 2
N1 Cu Cu 131.72(7) . 2
O7 Cu Cu 95.79(6) . 2
C6 N1 C2 114.6(3) . .
C6 N1 Cu 126.4(2) . .
C2 N1 Cu 117.6(2) . .
N2 C2 N3 118.1(3) . .
N2 C2 N1 117.4(3) . .
N3 C2 N1 124.5(3) . .
C2 N3 C4 114.9(3) . .
N4 C4 N5 117.0(3) . .
N4 C4 N3 117.6(3) . .
N5 C4 N3 125.4(3) . .
C6 N5 C4 115.3(3) . .
N6 C6 N5 117.8(3) . .
N6 C6 N1 117.7(3) . .
N5 C6 N1 124.4(3) . .
C7 O7 Cu 121.1(2) . .
C8 O8 Cu 125.8(2) . 2
C8 O8 Cu 122.5(2) . .
Cu O8 Cu 101.90(9) 2 .
O11 N9 O12 123.7(3) . .
O11 N9 O10 118.5(3) . .
O12 N9 O10 117.9(3) . .
N9 O10 Cu 110.3(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu O8 1.932(2) 2
Cu O8 1.933(2) .
Cu O10 1.996(2) .
Cu N1 2.010(2) .
Cu O7 2.426(2) .
Cu Cu 3.0018(8) 2
N1 C6 1.360(4) .
N1 C2 1.364(4) .
C2 N2 1.333(4) .
C2 N3 1.334(4) .
N3 C4 1.344(4) .
C4 N4 1.334(4) .
C4 N5 1.342(4) .
N5 C6 1.334(4) .
C6 N6 1.328(4) .
O7 C7 1.422(5) .
O8 C8 1.409(4) .
O8 Cu 1.932(2) 2
N9 O11 1.230(4) .
N9 O12 1.230(4) .
N9 O10 1.280(3) .
